Revisiting the hydrogenation behavior of NdGa and its hydride phases.
Shtender, Vitalii; Cedervall, Johan; Ek, Gustav; Zlotea, Claudia; Andersson, Mikael S.; Manuel, Pascal; Sahlberg, Martin; Häussermann, Ulrich; Journal of applied crystallography 57 (2024) 248–257; doi:10.1107/S1600576724000554

data_2300740
_publ_section_title
;
 Revisiting the hydrogenation behavior of NdGa and its hydride phases.
;
_journal_coeditor_code           NB5371
_journal_issue                   'Pt 2'
_journal_name_full               'Journal of applied crystallography'
_journal_page_first              248
_journal_page_last               257
_journal_paper_doi               10.1107/S1600576724000554
_journal_volume                  57
_journal_year                    2024
_chemical_formula_sum            'Ga3 Nd3'
_chemical_formula_weight         641.88
_space_group_crystal_system      orthorhombic
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_atom_sites_solution_primary     12
_audit_creation_method           SHELXL-2019/1
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.332(2)
_cell_length_b                   12.264(2)
_cell_length_c                   4.1782(7)
_cell_measurement_reflns_used    7329
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      39.415
_cell_measurement_theta_min      2.342
_cell_volume                     631.91(18)
_computing_structure_refinement  'SHELXL-2019/1 (Sheldrick, 2019)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measurement_device_type  'Bruker D8'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0306
_diffrn_reflns_av_unetI/netI     0.0217
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.989
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            7329
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.989
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         39.415
_diffrn_reflns_theta_min         2.342
_exptl_absorpt_coefficient_mu    36.650
_exptl_absorpt_correction_T_max  0.698
_exptl_absorpt_correction_T_min  0.641
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_density_diffrn    6.747
_exptl_crystal_description       needle
_exptl_crystal_F_000             1092
_exptl_crystal_size_max          0.03
_exptl_crystal_size_mid          0.01
_exptl_crystal_size_min          0.01
_refine_diff_density_max         4.216
_refine_diff_density_min         -3.410
_refine_diff_density_rms         0.521
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.080
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     21
_refine_ls_number_reflns         1070
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.080
_refine_ls_R_factor_all          0.0376
_refine_ls_R_factor_gt           0.0295
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0253P)^2^+17.8283P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0651
_refine_ls_wR_factor_ref         0.0683
_reflns_Friedel_coverage         0.000
_reflns_number_gt                919
_reflns_number_total             1070
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            nb5371sup1.cif
_cod_data_source_block           NdGaH1.6
_cod_depositor_comments
;Adding full bibliography for 2300736--2300740.cif.

 Adding full bibliography for 2300736--2300740.cif.
;
_cod_original_cell_volume        631.93(19)
_cod_database_code               2300740
_cod_database_fobs_code          2300740
_shelx_shelxl_version_number     2019/1
_shelx_res_checksum              56603
_shelx_hkl_checksum              66794